#------------------------------------------------------------------------------
#$Date: 2016-02-20 05:06:23 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176774 $
#$URL: svn://www.crystallography.net/cod/cif/2/20/70/2207082.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2207082
loop_
_publ_author_name
'Salloum, D.'
'Gougeon, P.'
'Potel, M.'
_publ_section_title
;
 Ag~1.91~Cs~1.16~Mo₉S₁₁: a novel quaternary reduced molybdenum
 sulfide containing Mo₉ clusters
;
_journal_coeditor_code           WM6090
_journal_issue                   10
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i213
_journal_page_last               i215
_journal_paper_doi               10.1107/S1600536805028205
_journal_volume                  61
_journal_year                    2005
_chemical_formula_iupac          'Ag1.91 Cs1.16 Mo9 S11'
_chemical_formula_structural     'Ag1.91 Cs1.16 (Mo9 S11)'
_chemical_formula_sum            'Ag1.91 Cs1.16 Mo9 S11'
_chemical_formula_weight         1576.99
_chemical_name_systematic
;
silver caesium nonamolybdenum undecasulfide
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_primary     isomor
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   9.63660(10)
_cell_length_b                   9.63660(10)
_cell_length_c                   11.6119(3)
_cell_measurement_reflns_used    13553
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      39.11
_cell_measurement_theta_min      1.70
_cell_volume                     933.86(3)
_computing_cell_refinement       COLLECT
_computing_data_collection       'COLLECT (Nonius, 1998)'
_computing_data_reduction        'EvalCCD (Duisenberg, 1998)'
_computing_molecular_graphics    'DIAMOND (Bergerhoff, 1996)'
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Nonius KappaCCD'
_diffrn_measurement_method       'φ scans and ω'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0385
_diffrn_reflns_av_sigmaI/netI    0.0233
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            16326
_diffrn_reflns_theta_full        39.76
_diffrn_reflns_theta_max         39.76
_diffrn_reflns_theta_min         3.01
_diffrn_standards_decay_%        0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    11.223
_exptl_absorpt_correction_T_max  0.5130
_exptl_absorpt_correction_T_min  0.3934
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(de Meulenaar & Tompa, 1965)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    5.608
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'truncated octahedron'
_exptl_crystal_F_000             1416
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.09
_refine_diff_density_max         1.275
_refine_diff_density_min         -1.315
_refine_ls_extinction_coef       0.00338(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL97
_refine_ls_goodness_of_fit_ref   1.081
_refine_ls_matrix_type           full
_refine_ls_number_parameters     50
_refine_ls_number_reflns         1982
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.081
_refine_ls_R_factor_all          0.0262
_refine_ls_R_factor_gt           0.0217
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w = 1/[σ²(Fo²)+(0.0146P)²+2.105P] where P = (Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0450
_refine_ls_wR_factor_ref         0.0457
_reflns_number_gt                1752
_reflns_number_total             1982
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            wm6090.cif
_cod_data_source_block           I
_cod_database_code               2207082
_cod_database_fobs_code          2207082
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-y, x-y, z'
'-x+y, -x, z'
'x-y, x, z+1/2'
'y, -x+y, z+1/2'
'-x, -y, -z'
'x, y, -z-1/2'
'y, -x+y, -z'
'x-y, x, -z'
'-x+y, -x, -z-1/2'
'-y, x-y, -z-1/2'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_type_symbol
Mo1 0.51582(2) 0.16899(2) 0.058863(14) 0.00800(4) Uani d . 1 Mo
Mo2 0.67583(3) 0.17495(3) 0.2500 0.00711(5) Uani d S 1 Mo
S1 0.35745(6) 0.30591(6) 0.06805(4) 0.01006(9) Uani d . 1 S
S2 0.38169(9) 0.03069(9) 0.2500 0.01058(12) Uani d S 1 S
S3 0.6667 0.3333 -0.10280(8) 0.01318(15) Uani d S 1 S
Ag 0.57939(6) -0.16398(5) 0.2500 0.02623(15) Uani d SP 0.636(2) Ag
Cs1 0.0000 0.0000 0.2500 0.139(5) Uani d SP 0.573(15) Cs
Cs2 0.0000 0.0000 0.4029(18) 0.176(8) Uani d SP 0.294(8) Cs
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
S3 Mo1 S1 . . 90.767(13)
S3 Mo1 S1 . 3_655 90.316(13)
S1 Mo1 S1 . 3_655 173.41(2)
S3 Mo1 S1 . 9 93.662(19)
S1 Mo1 S1 . 9 91.47(2)
S1 Mo1 S1 3_655 9 94.947(17)
S3 Mo1 S2 . . 171.42(2)
S1 Mo1 S2 . . 87.42(2)
S1 Mo1 S2 3_655 . 90.55(2)
S1 Mo1 S2 9 . 94.766(19)
S3 Mo1 Mo1 . 4_665 56.935(11)
S1 Mo1 Mo1 . 4_665 58.196(14)
S1 Mo1 Mo1 3_655 4_665 117.442(14)
S1 Mo1 Mo1 9 4_665 133.873(14)
S2 Mo1 Mo1 . 4_665 115.366(16)
S3 Mo1 Mo1 . 3_655 56.935(11)
S1 Mo1 Mo1 . 3_655 118.134(14)
S1 Mo1 Mo1 3_655 3_655 57.503(14)
S1 Mo1 Mo1 9 3_655 135.936(13)
S2 Mo1 Mo1 . 3_655 116.908(15)
Mo1 Mo1 Mo1 4_665 3_655 60.0
S3 Mo1 Mo2 . . 118.478(13)
S1 Mo1 Mo2 . . 117.028(14)
S1 Mo1 Mo2 3_655 . 56.959(13)
S1 Mo1 Mo2 9 . 134.752(14)
S2 Mo1 Mo2 . . 55.533(16)
Mo1 Mo1 Mo2 4_665 . 91.328(6)
Mo1 Mo1 Mo2 3_655 . 61.573(7)
S3 Mo1 Mo2 . 4_665 117.007(14)
S1 Mo1 Mo2 . 4_665 56.616(13)
S1 Mo1 Mo2 3_655 4_665 117.281(14)
S1 Mo1 Mo2 9 4_665 133.564(15)
S2 Mo1 Mo2 . 4_665 55.311(16)
Mo1 Mo1 Mo2 4_665 4_665 60.100(6)
Mo1 Mo1 Mo2 3_655 4_665 90.472(6)
Mo2 Mo1 Mo2 . 4_665 60.413(9)
S3 Mo1 Mo1 . 7_655 92.971(12)
S1 Mo1 Mo1 . 7_655 138.201(15)
S1 Mo1 Mo1 3_655 7_655 48.195(12)
S1 Mo1 Mo1 9 7_655 46.752(12)
S2 Mo1 Mo1 . 7_655 93.968(17)
Mo1 Mo1 Mo1 4_665 7_655 148.814(8)
Mo1 Mo1 Mo1 3_655 7_655 98.328(11)
Mo2 Mo1 Mo1 . 7_655 97.361(8)
Mo2 Mo1 Mo1 4_665 7_655 148.292(10)
S3 Mo1 Ag . 7_655 47.083(15)
S1 Mo1 Ag . 7_655 80.398(15)
S1 Mo1 Ag 3_655 7_655 105.012(15)
S1 Mo1 Ag 9 7_655 48.621(14)
S2 Mo1 Ag . 7_655 140.474(17)
Mo1 Mo1 Ag 4_665 7_655 89.624(8)
Mo1 Mo1 Ag 3_655 7_655 101.897(8)
Mo2 Mo1 Ag . 7_655 159.697(11)
Mo2 Mo1 Ag 4_665 7_655 135.639(10)
Mo1 Mo1 Ag 7_655 7_655 72.229(9)
S3 Mo1 Mo2 . 3_655 86.599(14)
S1 Mo1 Mo2 . 3_655 87.663(13)
S1 Mo1 Mo2 3_655 3_655 85.913(13)
S1 Mo1 Mo2 9 3_655 179.099(14)
S2 Mo1 Mo2 . 3_655 84.950(15)
Mo1 Mo1 Mo2 4_665 3_655 45.695(4)
Mo1 Mo1 Mo2 3_655 3_655 44.852(4)
Mo2 Mo1 Mo2 . 3_655 45.645(6)
Mo2 Mo1 Mo2 4_665 3_655 45.632(6)
Mo1 Mo1 Mo2 7_655 3_655 134.107(9)
Ag Mo1 Mo2 7_655 3_655 131.401(9)
S3 Mo1 Ag . . 129.991(9)
S1 Mo1 Ag . . 138.797(14)
S1 Mo1 Ag 3_655 . 39.675(14)
S1 Mo1 Ag 9 . 91.533(14)
S2 Mo1 Ag . . 51.381(18)
Mo1 Mo1 Ag 4_665 . 134.457(8)
Mo1 Mo1 Ag 3_655 . 86.317(10)
Mo2 Mo1 Ag . . 43.682(7)
Mo2 Mo1 Ag 4_665 . 93.447(7)
Mo1 Mo1 Ag 7_655 . 57.132(6)
Ag Mo1 Ag 7_655 . 129.361(6)
Mo2 Mo1 Ag 3_655 . 88.957(7)
S3 Mo1 S3 . 7_655 127.354(6)
S1 Mo1 S3 . 7_655 125.862(13)
S1 Mo1 S3 3_655 7_655 57.743(12)
S1 Mo1 S3 9 7_655 54.445(15)
S2 Mo1 S3 . 7_655 59.730(19)
Mo1 Mo1 S3 4_665 7_655 171.677(11)
Mo1 Mo1 S3 3_655 7_655 115.075(8)
Mo2 Mo1 S3 . 7_655 80.349(12)
Mo2 Mo1 S3 4_665 7_655 114.859(13)
Mo1 Mo1 S3 7_655 7_655 34.383(11)
Ag Mo1 S3 7_655 7_655 98.170(14)
Mo2 Mo1 S3 3_655 7_655 125.983(11)
Ag Mo1 S3 . 7_655 37.307(10)
S3 Mo1 S1 . 4_665 52.347(15)
S1 Mo1 S1 . 4_665 87.873(8)
S1 Mo1 S1 3_655 4_665 87.644(8)
S1 Mo1 S1 9 4_665 145.971(9)
S2 Mo1 S1 . 4_665 119.170(16)
Mo1 Mo1 S1 4_665 4_665 29.798(8)
Mo1 Mo1 S1 3_655 4_665 30.261(8)
Mo2 Mo1 S1 . 4_665 73.770(9)
Mo2 Mo1 S1 4_665 4_665 72.252(9)
Mo1 Mo1 S1 7_655 4_665 126.158(10)
Ag Mo1 S1 7_655 4_665 97.930(11)
Mo2 Mo1 S1 3_655 4_665 34.262(7)
Ag Mo1 S1 . 4_665 110.937(10)
S3 Mo1 S1 7_655 4_665 144.595(8)
S3 Mo1 Ag . 3_545 159.014(15)
S1 Mo1 Ag . 3_545 94.721(15)
S1 Mo1 Ag 3_655 3_545 86.546(14)
S1 Mo1 Ag 9 3_545 66.003(13)
S2 Mo1 Ag . 3_545 29.556(14)
Mo1 Mo1 Ag 4_665 3_545 141.538(8)
Mo1 Mo1 Ag 3_655 3_545 134.938(9)
Mo2 Mo1 Ag . 3_545 76.681(7)
Mo2 Mo1 Ag 4_665 3_545 82.602(8)
Mo1 Mo1 Ag 7_655 3_545 69.615(8)
Ag Mo1 Ag 7_655 3_545 114.012(11)
Mo2 Mo1 Ag 3_655 3_545 113.814(5)
Ag Mo1 Ag . 3_545 50.079(14)
S3 Mo1 Ag 7_655 3_545 36.367(10)
S1 Mo1 Ag 4_665 3_545 147.955(8)
S2 Mo2 S2 . 3_655 172.79(2)
S2 Mo2 S1 . 12_656 93.858(16)
S2 Mo2 S1 3_655 12_656 89.883(16)
S2 Mo2 S1 . 3_655 93.858(16)
S2 Mo2 S1 3_655 3_655 89.883(16)
S1 Mo2 S1 12_656 3_655 117.33(3)
S2 Mo2 Mo1 . . 60.004(8)
S2 Mo2 Mo1 3_655 . 117.603(9)
S1 Mo2 Mo1 12_656 . 150.850(16)
S1 Mo2 Mo1 3_655 . 57.464(13)
S2 Mo2 Mo1 . 8_556 60.004(8)
S2 Mo2 Mo1 3_655 8_556 117.603(9)
S1 Mo2 Mo1 12_656 8_556 57.464(13)
S1 Mo2 Mo1 3_655 8_556 150.850(16)
Mo1 Mo2 Mo1 . 8_556 111.397(11)
S2 Mo2 Mo2 . 3_655 116.58(2)
S2 Mo2 Mo2 3_655 3_655 56.21(2)
S1 Mo2 Mo2 12_656 3_655 115.536(14)
S1 Mo2 Mo2 3_655 3_655 115.536(14)
Mo1 Mo2 Mo2 . 3_655 89.490(6)
Mo1 Mo2 Mo2 8_556 3_655 89.490(6)
S2 Mo2 Mo2 . 4_665 56.58(2)
S2 Mo2 Mo2 3_655 4_665 116.21(2)
S1 Mo2 Mo2 12_656 4_665 117.870(14)
S1 Mo2 Mo2 3_655 4_665 117.870(14)
Mo1 Mo2 Mo2 . 4_665 60.499(7)
Mo1 Mo2 Mo2 8_556 4_665 60.499(7)
Mo2 Mo2 Mo2 3_655 4_665 60.0
S2 Mo2 Mo1 . 12_656 118.128(9)
S2 Mo2 Mo1 3_655 12_656 59.323(8)
S1 Mo2 Mo1 12_656 12_656 56.450(13)
S1 Mo2 Mo1 3_655 12_656 146.973(16)
Mo1 Mo2 Mo1 . 12_656 145.118(10)
Mo1 Mo2 Mo1 8_556 12_656 58.327(7)
Mo2 Mo2 Mo1 3_655 12_656 59.088(7)
Mo2 Mo2 Mo1 4_665 12_656 88.686(6)
S2 Mo2 Mo1 . 3_655 118.128(9)
S2 Mo2 Mo1 3_655 3_655 59.323(8)
S1 Mo2 Mo1 12_656 3_655 146.973(16)
S1 Mo2 Mo1 3_655 3_655 56.450(13)
Mo1 Mo2 Mo1 . 3_655 58.327(7)
Mo1 Mo2 Mo1 8_556 3_655 145.118(10)
Mo2 Mo2 Mo1 3_655 3_655 59.088(7)
Mo2 Mo2 Mo1 4_665 3_655 88.686(6)
Mo1 Mo2 Mo1 12_656 3_655 109.041(11)
S2 Mo2 Ag . . 74.60(2)
S2 Mo2 Ag 3_655 . 112.61(2)
S1 Mo2 Ag 12_656 . 61.360(13)
S1 Mo2 Ag 3_655 . 61.360(13)
Mo1 Mo2 Ag . . 96.777(9)
Mo1 Mo2 Ag 8_556 . 96.777(9)
Mo2 Mo2 Ag 3_655 . 168.818(17)
Mo2 Mo2 Ag 4_665 . 131.182(17)
Mo1 Mo2 Ag 12_656 . 116.846(8)
Mo1 Mo2 Ag 3_655 . 116.846(8)
S2 Mo2 Mo1 . 11_666 86.642(16)
S2 Mo2 Mo1 3_655 11_666 87.502(15)
S1 Mo2 Mo1 12_656 11_666 85.649(13)
S1 Mo2 Mo1 3_655 11_666 156.879(14)
Mo1 Mo2 Mo1 . 11_666 103.965(8)
Mo1 Mo2 Mo1 8_556 11_666 43.820(5)
Mo2 Mo2 Mo1 3_655 11_666 45.682(4)
Mo2 Mo2 Mo1 4_665 11_666 44.865(4)
Mo1 Mo2 Mo1 12_656 11_666 43.833(5)
Mo1 Mo2 Mo1 3_655 11_666 103.166(7)
Ag Mo2 Mo1 . 11_666 139.984(7)
Mo1 S1 Mo2 . 4_665 66.934(14)
Mo1 S1 Mo1 . 4_665 64.301(15)
Mo2 S1 Mo1 4_665 4_665 65.577(14)
Mo1 S1 Mo1 . 10 132.91(2)
Mo2 S1 Mo1 4_665 10 132.69(2)
Mo1 S1 Mo1 4_665 10 85.053(17)
Mo1 S1 Ag . 4_665 132.75(2)
Mo2 S1 Ag 4_665 4_665 67.178(15)
Mo1 S1 Ag 4_665 4_665 105.42(2)
Mo1 S1 Ag 10 4_665 87.886(18)
Mo1 S1 Cs2 . 8_556 100.262(19)
Mo2 S1 Cs2 4_665 8_556 105.9(3)
Mo1 S1 Cs2 4_665 8_556 164.08(8)
Mo1 S1 Cs2 10 8_556 109.6(2)
Ag S1 Cs2 4_665 8_556 81.9(3)
Mo1 S1 Cs2 . 2_554 97.35(4)
Mo2 S1 Cs2 4_665 2_554 138.6(2)
Mo1 S1 Cs2 4_665 2_554 143.6(3)
Mo1 S1 Cs2 10 2_554 86.70(18)
Ag S1 Cs2 4_665 2_554 109.6(2)
Cs2 S1 Cs2 8_556 2_554 36.7(7)
Mo1 S1 Cs1 . . 99.773(16)
Mo2 S1 Cs1 4_665 . 80.599(14)
Mo1 S1 Cs1 4_665 . 145.951(19)
Mo1 S1 Cs1 10 . 123.317(17)
Ag S1 Cs1 4_665 . 62.002(15)
Cs2 S1 Cs1 8_556 . 27.3(4)
Cs2 S1 Cs1 2_554 . 64.0(3)
Mo1 S1 Mo1 . 3_655 32.068(8)
Mo2 S1 Mo1 4_665 3_655 60.088(11)
Mo1 S1 Mo1 4_665 3_655 32.297(8)
Mo1 S1 Mo1 10 3_655 111.611(16)
Ag S1 Mo1 4_665 3_655 122.614(18)
Cs2 S1 Mo1 8_556 3_655 132.03(3)
Cs2 S1 Mo1 2_554 3_655 124.33(12)
Cs1 S1 Mo1 . 3_655 125.054(13)
Mo2 S2 Mo2 . 4_665 67.21(2)
Mo2 S2 Ag . 3_545 135.94(4)
Mo2 S2 Ag 4_665 3_545 156.85(4)
Mo2 S2 Mo1 . 8_556 64.462(15)
Mo2 S2 Mo1 4_665 8_556 65.366(16)
Ag S2 Mo1 3_545 8_556 119.883(15)
Mo2 S2 Mo1 . . 64.462(15)
Mo2 S2 Mo1 4_665 . 65.366(16)
Ag S2 Mo1 3_545 . 119.883(15)
Mo1 S2 Mo1 8_556 . 118.78(3)
Mo2 S2 Cs1 . . 154.78(3)
Mo2 S2 Cs1 4_665 . 87.57(2)
Ag S2 Cs1 3_545 . 69.28(2)
Mo1 S2 Cs1 8_556 . 105.936(18)
Mo1 S2 Cs1 . . 105.936(18)
Mo2 S2 Cs2 . 8_556 143.97(19)
Mo2 S2 Cs2 4_665 8_556 87.83(2)
Ag S2 Cs2 3_545 8_556 71.56(5)
Mo1 S2 Cs2 8_556 8_556 129.1(2)
Mo1 S2 Cs2 . 8_556 81.9(2)
Cs1 S2 Cs2 . 8_556 26.6(3)
Mo2 S2 Cs2 . . 143.97(19)
Mo2 S2 Cs2 4_665 . 87.83(2)
Ag S2 Cs2 3_545 . 71.56(5)
Mo1 S2 Cs2 8_556 . 81.9(2)
Mo1 S2 Cs2 . . 129.1(2)
Cs1 S2 Cs2 . . 26.6(3)
Cs2 S2 Cs2 8_556 . 53.3(6)
Mo2 S2 Mo1 . 11_666 59.586(13)
Mo2 S2 Mo1 4_665 11_666 32.688(7)
Ag S2 Mo1 3_545 11_666 148.289(10)
Mo1 S2 Mo1 8_556 11_666 32.726(11)
Mo1 S2 Mo1 . 11_666 91.451(19)
Cs1 S2 Mo1 . 11_666 99.188(16)
Cs2 S2 Mo1 8_556 11_666 111.62(11)
Cs2 S2 Mo1 . 11_666 85.24(15)
Mo2 S2 Mo1 . 4_665 59.586(13)
Mo2 S2 Mo1 4_665 4_665 32.688(7)
Ag S2 Mo1 3_545 4_665 148.289(9)
Mo1 S2 Mo1 8_556 4_665 91.451(19)
Mo1 S2 Mo1 . 4_665 32.726(11)
Cs1 S2 Mo1 . 4_665 99.188(16)
Cs2 S2 Mo1 8_556 4_665 85.24(14)
Cs2 S2 Mo1 . 4_665 111.62(11)
Mo1 S2 Mo1 11_666 4_665 60.456(11)
Mo2 S2 Mo1 . 2_655 78.462(13)
Mo2 S2 Mo1 4_665 2_655 115.221(13)
Ag S2 Mo1 3_545 2_655 76.342(14)
Mo1 S2 Mo1 8_556 2_655 50.338(10)
Mo1 S2 Mo1 . 2_655 139.63(2)
Cs1 S2 Mo1 . 2_655 114.437(11)
Cs2 S2 Mo1 8_556 2_655 137.3(2)
Cs2 S2 Mo1 . 2_655 90.3(3)
Mo1 S2 Mo1 11_666 2_655 82.629(6)
Mo1 S2 Mo1 4_665 2_655 133.686(16)
Mo2 S2 Mo1 . 7_655 78.462(13)
Mo2 S2 Mo1 4_665 7_655 115.221(13)
Ag S2 Mo1 3_545 7_655 76.342(14)
Mo1 S2 Mo1 8_556 7_655 139.63(2)
Mo1 S2 Mo1 . 7_655 50.338(10)
Cs1 S2 Mo1 . 7_655 114.437(11)
Cs2 S2 Mo1 8_556 7_655 90.3(3)
Cs2 S2 Mo1 . 7_655 137.3(2)
Mo1 S2 Mo1 11_666 7_655 133.686(16)
Mo1 S2 Mo1 4_665 7_655 82.629(6)
Mo1 S2 Mo1 2_655 7_655 108.857(17)
Mo1 S3 Mo1 3_655 . 66.13(2)
Mo1 S3 Mo1 3_655 4_665 66.13(2)
Mo1 S3 Mo1 . 4_665 66.13(2)
Mo1 S3 Ag 3_655 9_665 92.109(8)
Mo1 S3 Ag . 9_665 123.937(11)
Mo1 S3 Ag 4_665 9_665 151.048(14)
Mo1 S3 Ag 3_655 7_655 151.048(14)
Mo1 S3 Ag . 7_655 92.109(8)
Mo1 S3 Ag 4_665 7_655 123.937(11)
Ag S3 Ag 9_665 7_655 84.42(2)
Mo1 S3 Ag 3_655 10 123.937(11)
Mo1 S3 Ag . 10 151.048(14)
Mo1 S3 Ag 4_665 10 92.109(8)
Ag S3 Ag 9_665 10 84.42(2)
Ag S3 Ag 7_655 10 84.42(2)
Mo1 S3 Mo1 3_655 9_665 52.646(6)
Mo1 S3 Mo1 . 9_665 118.23(2)
Mo1 S3 Mo1 4_665 9_665 81.704(11)
Ag S3 Mo1 9_665 9_665 69.665(9)
Ag S3 Mo1 7_655 9_665 147.59(3)
Ag S3 Mo1 10 9_665 74.286(10)
Mo1 S3 Mo1 3_655 7_655 81.704(11)
Mo1 S3 Mo1 . 7_655 52.646(6)
Mo1 S3 Mo1 4_665 7_655 118.23(2)
Ag S3 Mo1 9_665 7_655 74.286(10)
Ag S3 Mo1 7_655 7_655 69.665(9)
Ag S3 Mo1 10 7_655 147.59(3)
Mo1 S3 Mo1 9_665 7_655 118.596(5)
Mo1 S3 Mo1 3_655 10 118.23(2)
Mo1 S3 Mo1 . 10 81.704(11)
Mo1 S3 Mo1 4_665 10 52.646(6)
Ag S3 Mo1 9_665 10 147.59(3)
Ag S3 Mo1 7_655 10 74.286(10)
Ag S3 Mo1 10 10 69.665(9)
Mo1 S3 Mo1 9_665 10 118.596(5)
Mo1 S3 Mo1 7_655 10 118.596(5)
S2 Ag S3 4_655 7_655 90.901(18)
S2 Ag S3 4_655 2_655 90.901(18)
S3 Ag S3 7_655 2_655 78.25(3)
S2 Ag S1 4_655 12_656 117.004(19)
S3 Ag S1 7_655 12_656 146.34(2)
S3 Ag S1 2_655 12_656 82.624(17)
S2 Ag S1 4_655 3_655 117.004(19)
S3 Ag S1 7_655 3_655 82.624(17)
S3 Ag S1 2_655 3_655 146.34(2)
S1 Ag S1 12_656 3_655 99.15(2)
S2 Cs1 S2 4 . 120.0
S2 Cs1 S2 4 3 120.0
S2 Cs1 S2 . 3 120.0
S2 Cs1 S1 4 8_556 144.962(8)
S2 Cs1 S1 . 8_556 56.104(12)
S2 Cs1 S1 3 8_556 74.866(12)
S2 Cs1 S1 4 3 74.866(12)
S2 Cs1 S1 . 3 144.962(8)
S2 Cs1 S1 3 3 56.104(12)
S1 Cs1 S1 8_556 3 130.553(5)
S2 Cs1 S1 4 12_556 74.866(12)
S2 Cs1 S1 . 12_556 144.962(8)
S2 Cs1 S1 3 12_556 56.104(12)
S1 Cs1 S1 8_556 12_556 92.841(11)
S1 Cs1 S1 3 12_556 66.458(15)
S2 Cs1 S1 4 4 56.104(12)
S2 Cs1 S1 . 4 74.866(12)
S2 Cs1 S1 3 4 144.962(8)
S1 Cs1 S1 8_556 4 130.553(5)
S1 Cs1 S1 3 4 92.841(11)
S1 Cs1 S1 12_556 4 130.553(5)
S1 Cs2 S1 8_556 12_556 118.93(13)
S1 Cs2 S1 8_556 11_556 118.93(13)
S1 Cs2 S1 12_556 11_556 118.93(13)
S1 Cs2 S1 8_556 5 61.27(15)
S1 Cs2 S1 12_556 5 61.27(15)
S1 Cs2 S1 11_556 5 143.3(7)
S1 Cs2 S1 8_556 6 61.27(15)
S1 Cs2 S1 12_556 6 143.3(7)
S1 Cs2 S1 11_556 6 61.27(15)
S1 Cs2 S1 5 6 96.2(4)
S1 Cs2 S1 8_556 2 143.3(7)
S1 Cs2 S1 12_556 2 61.27(15)
S1 Cs2 S1 11_556 2 61.27(15)
S1 Cs2 S1 5 2 96.2(4)
S1 Cs2 S1 6 2 96.2(4)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Mo1 S3 . 2.4172(7) y
Mo1 S1 . 2.4688(5) y
Mo1 S1 3_655 2.4877(5) y
Mo1 S1 9 2.5458(5) y
Mo1 S2 . 2.5788(4) y
Mo1 Mo1 4_665 2.6376(3) y
Mo1 Mo1 3_655 2.6376(3) ?
Mo1 Mo2 . 2.6867(2) y
Mo1 Mo2 4_665 2.7255(2) y
Mo1 Mo1 7_655 3.4025(3) ?
Mo1 Ag 7_655 3.6963(2) ?
Mo1 Mo2 3_655 3.8084(2) ?
Mo1 Ag . 4.1908(4) ?
Mo1 S3 7_655 4.2747(2) ?
Mo1 S1 4_665 4.3810(5) ?
Mo1 Ag 3_545 4.3975(4) ?
Mo2 S2 . 2.4549(8) y
Mo2 S2 3_655 2.4654(8) y
Mo2 S1 12_656 2.4736(5) y
Mo2 S1 3_655 2.4736(5) y
Mo2 Mo1 8_556 2.6867(2) ?
Mo2 Mo2 3_655 2.7232(4) y
Mo2 Mo2 4_665 2.7232(4) ?
Mo2 Mo1 12_656 2.7255(2) ?
Mo2 Mo1 3_655 2.7255(2) ?
Mo2 Ag . 2.9148(5) ?
Mo2 Mo1 11_666 3.8084(2) ?
S1 Mo2 4_665 2.4736(5) ?
S1 Mo1 4_665 2.4877(5) ?
S1 Mo1 10 2.5458(5) ?
S1 Ag 4_665 2.7754(6) ?
S1 Cs2 8_556 3.243(2) ?
S1 Cs2 2_554 3.752(11) ?
S1 Cs1 . 3.8555(5) ?
S1 Mo1 3_655 4.3810(5) ?
S2 Mo2 4_665 2.4654(8) ?
S2 Ag 3_545 2.5018(8) ?
S2 Mo1 8_556 2.5788(4) ?
S2 Cs1 . 3.5396(7) ?
S2 Cs2 8_556 3.960(10) ?
S2 Cs2 . 3.960(10) ?
S2 Mo1 11_666 4.4085(7) ?
S2 Mo1 4_665 4.4085(7) ?
S2 Mo1 2_655 4.4093(5) ?
S2 Mo1 7_655 4.4093(5) ?
S3 Mo1 3_655 2.4172(7) ?
S3 Mo1 4_665 2.4172(7) ?
S3 Ag 9_665 2.7088(7) ?
S3 Ag 7_655 2.7088(7) ?
S3 Ag 10 2.7088(7) ?
S3 Mo1 9_665 4.2747(2) ?
S3 Mo1 7_655 4.2747(2) ?
S3 Mo1 10 4.2747(2) ?
Ag S2 4_655 2.5018(8) y
Ag S3 7_655 2.7088(7) y
Ag S3 2_655 2.7088(7) y
Ag S1 12_656 2.7754(6) y
Ag S1 3_655 2.7754(6) y
Ag Cs1 1_655 3.5385(5) ?
Ag Mo1 2_655 3.6963(2) ?
Ag Mo1 7_655 3.6963(2) ?
Ag Cs2 1_655 3.959(10) ?
Ag Cs2 8_656 3.959(10) ?
Ag Mo1 8_556 4.1908(4) ?
Cs1 Cs2 . 1.78(2) ?
Cs1 Cs2 8_556 1.78(2) ?
Cs1 Ag 4_665 3.5385(5) ?
Cs1 Ag 1_455 3.5385(5) ?
Cs1 Ag 3_545 3.5385(5) ?
Cs1 S2 4 3.5396(7) y
Cs1 S2 3 3.5396(7) ?
Cs1 S1 8_556 3.8555(5) y
Cs1 S1 3 3.8555(5) ?
Cs1 S1 12_556 3.8555(5) ?
Cs1 S1 4 3.8555(5) ?
Cs1 S1 11_556 3.8555(5) ?
Cs1 Cs2 2_554 4.03(2) ?
Cs1 Cs2 7_556 4.03(2) ?
Cs1 Mo2 4_665 4.2270(2) ?
Cs1 Mo2 3_545 4.2270(2) ?
Cs1 Mo2 1_455 4.2270(2) ?
Cs1 S1 5 4.9031(5) ?
Cs2 Cs2 7_556 2.26(4) ?
Cs2 S1 8_556 3.243(2) y
Cs2 S1 12_556 3.243(2) ?
Cs2 S1 11_556 3.243(2) ?
Cs2 Cs2 8_556 3.55(4) ?
Cs2 S1 5 3.752(11) y
Cs2 S1 6 3.752(11) ?
Cs2 S1 2 3.752(11) ?
Cs2 Ag 1_455 3.959(10) ?
Cs2 Ag 4_665 3.959(10) ?
Cs2 Ag 3_545 3.959(10) ?
Cs2 S2 4 3.960(10) y
Cs2 S2 3 3.960(10) ?
Cs2 Cs1 7_556 4.03(2) ?
Cs2 Mo1 12_556 4.412(2) ?
Cs2 Mo1 11_556 4.412(2) ?
Cs2 Mo1 8_556 4.412(2) ?
Cs2 Mo2 3_545 4.585(8) ?
